EPDM Rubber Tile Soft fall Surfacing.
EDPM Rubber Granule Soft fall Surfacing - is one of the best soft fall available for commercial playground equipment. It is structurally stable ensuring you will always comply with Australian Safety standards regarding rubber soft fall surfacing. Schools, councils and commercial businesses with playground equipment are best off using rubber soft fall tiles for both ease of fixing if it is vandalised and ofcourse safety!
Existing Areas No Problems !
Laid on Concrete Or Crushed Rock !
EDPM Rubber Granule Soft fall - One of the highest quality of soft fall surfacing for commercial playground equipment, fitness areas and general activity venues.
Rubber soft fall is
structurally stable ensuring you will always comply with
Australian Safety standards regarding soft fall surfacing.
Please contact us for further information, specifications and costing's. All of our prices include crushed rock base, surface
installation and surrounds. Pricing assumes a clear and level site
with adequate drainage.
Would you like visit our referral's section to see some of our rubber soft fall supplied and installed.
Or just simply return to the home page to see our huge range of playground equipment and shade structures.
PLEASE REFER BELOW FOR THE PLAYGROUND SAFETY SURFACE TEST REPORT
School of Mechanical Engineering
The University of Adelaide
1.0 Executive Summary
ImaginationPlay provide a tiled dual-layer wet-pour recycled EPDM/rubber granule product for assessment as
playground undersurfacing material. The test was conducted on the impact absorption properties of the tiled
rubber undersurfacing product according to the impact test requirements of the Australian Standard:
AS4422:1996, when glued together in the manner specified by the manufacturer.
The impact test result for this
product sample is listed in Table 1 below.
Product Combination (Nominal Thickness) Critical Fall Height (m)
“EDPM” Rubber Impact Surface Tile (50mm) 1.4
Table 1: Critical Fall Height for the thickness configuration tested.
The impact absorption properties of a wet-pour recycled rubber tile product as supplied by ImaginationPlay was
measured according to the impact test requirements specified by the Australian Standard AS/NZS 4422:1996.
The sample consisted of four separate dual rubber layer test pieces, glued together along common edges, resulting with a
combined test piece of size of 1m × 1m.
The testing involved dropping a 5 kg anatomically-shaped aluminium headform from specified heights and
measuring the deceleration of the headform as it strikes the test samples. The severity of the impact is measured
in terms of the Head Injury Criterion (HIC).
The Australian Standard AS/NZS 4422:1996 concentrates on a method for measurement of HIC, which indicates
the deceleration impact on the brain. It is does not indicate injury potential to other parts of the body. The HIC
values set in the standard are those, which, if exceeded, are likely to result in injury to the brain. It should be
noted that although the standard stipulates that a HIC value of 1000 (or a deceleration value of 200 g) will
determine the critical fall height, this does not have widespread agreement. Common sense should always be
used in the interpretation and implementation of the results.
3.0 Referenced Documents
The documents that are pertinent to this report are:
• Australian Standard AS/NZS 4422:1996, “Playground surfacing - Specifications, requirements and test
• Australian Standard AS/NZS 4422:1996, “Playground surfacing - Specifications, requirements and test
• Australian Standard AS 2512.1:1996, “Methods of testing protective helmets”.
• International Standards Organization ISO 6487, “Road vehicles-measurement techniques in impact tests -
4.0 Equipment and Procedure
The equipment used in the experimental testing is shown in Figure 1.
The equipment that was used to perform the impact testing is outlined below:
Drop Rig: The testing drop rig is a portable stand that is used to raise the headform. A pin is
released which permits the headform to fall unguided onto the test sample. The height
to which the headform is raised is measured with a vertical measuring tape between
the upper surface of the sample and the lowest point of the hanging headform.
Headform: The headform is made from aluminium and has an anatomical shape that complies
with the J-Type headform from AS 2512.1. It has a mass of 5.1kg. A tri-axial
accelerometer (Endevco 7268C-2000) is mounted at the centre of gravity of the
headform. The frequency range of the accelerometers is from 0-1000Hz. This
complies with channel class 1000 of ISO 6487. A cable connects the tri-axial
accelerometer to the strain gauge amplifiers.
Strain Gauge Amplifiers: The 3-channel Endevco Model 136 DC strain gauge amplifier is configured for fullbridge
circuit configurations. High precision balancing resistors are used to convert the half-bridge accelerometers into a full-bridge circuit. Anti-aliasing filters (at
10kHz) are used for each channel.
Recording Equipment: The output from the strain gauge amplifiers is connected to an analog to digital (A/D)
converter board inside a notebook portable computer. The A/D board samples at
20.0kHz. The collection of data is triggered automatically based on the starting point
of an impact event as determined from the constant monitoring of a selected channel
value. The data acquisition procedure has a pre-trigger capability, such that the data is
collected over a time period spanning from just before to just after the impact event. A
sine wave at 200Hz is supplied to one of the A/D channels to provide a check that the
sampling rate is accurate.
Product Sample: The tiled sample rubber soft fall undersurfacing material was supplied in the form of four
(equal) pieces glued together (by the manufacturer), with a total size of 1m × 1m.
This was positioned flat against a concrete floor.
All testing was conducted at the Thebarton Campus of the University of Adelaide in a laboratory environment.
The testing method follows the Australian Standard AS/NZS 4422:1996. In general terms, the sample to be
tested was placed on a concrete floor beneath the drop testing rig, the J-type headform was released from various
heights and the deceleration of the headform was measured as it struck the test sample. The critical fall height is
determined as the height when the Head Injury Criteria (HIC) equals 1000. The Head Injury Criteria is
a = the dimensionless ratio of the deceleration experienced by the headform to the deceleration due to
gravity (in g).
t2 , t1 = instant of time during the impact, chosen such that HIC is maximised, where t2 > t1.
The critical fall height is the height at which the HIC equals 1000 (or deceleration equals 200 g), rounded down
to the nearest 10cm, as specified in AS/NZS 4422:1996.
The test procedure is listed below:
- Prior to testing, the manufacturer’s calibration values for the tri-axial accelerometer are checked by aligning
each axis in a vertical direction so that a voltage measurement can be obtained for positive and negative
accelerations due to gravity.
- The acceleration measurement obtained using the instrumented headform is verified by dropping it onto a
standard rubber mat, both before and after testing, to ensure consistency and accuracy of data measurement.
- The test rubber soft fall sample is placed beneath the headform.
- The headform is raised and held in position. The vertical height between the test sample and the lowest part
of the headform is measured with a vertical tape measure.
- The headform is released and is allowed to fall unguided and strike the test sample. The collection of data on
the A/D board is triggered based on the beginning of the impact event. Data is collected from just before to
just after the impact event.
- The data is analysed to determine the HIC value and Maximum g value for the drop test.
- Steps 4-6 are then repeated so that a HIC value is obtained for each of four separate heights at the same
location on the test sample. The heights are selected so that HIC values are determined below 1000, close to
1000 and above 1000 (or alternatively, deceleration values below 200 g, close to 200 g and above 200 g).
For some cases with the present product combinations, it was found necessary to drop the headform three
times at the test location prior to beginning the test measurements (see note below).
- The headform impact location on the test sample is moved to a new position. A total of three separate test
positions are selected for tile surfacing materials. The test positions for tiled surfaces correspond with one
location in the middle of the tile surface, one location on the join between two tiles, and one location on the
join between all four tiles.
- Graphs are drawn of the HIC values versus the drop height. The critical fall height is determined by the
height at which the HIC value equals 1000 (or deceleration equals 200 g), rounded down to the nearest 10cm.
The surfacing samples were tested at the locations shown in the Test Sheets in the Appendix.
Note: For the dual-layer rubber product samples tested, the magnitudes of the impact results over the first three
drops (at any particular location) were found to be increasing. Since the impact performance of the surfaces
during these three drops were generally non-repeatable, it is deemed not appropriate to include these initial
results among those to be considered for the AS4422:1996 standard. They do not provide a good indication of
the longer term (repeatable) performances of the rubber undersurfacing surfaces, and are generally not included
on this basis. The impact test results measured after this initial “conditioning” process were found to be
reasonably consistent and repeatable within acceptable limits.
““EDPM” Rubber Impact Surface Tile (50mm)”
According to the manufacturer, the EPDM/recycled rubber impact surface tiles are described as follows:
“The top-coat surface layer consists of EPDM rubber granules of approximate diameter of 1mm, and
has a thickness of 10mm. The 40mm thick base layer is made from shredded and granulated recycled
tyre rubber particles of varying specified sizes. All particles in both layers are bonded together with a
“EDPM” Rubber Impact Surface Tile (50mm) Undersurfacing Product
A photograph of the ‘“EDPM” Rubber Impact Surface Tile (50mm)’ undersurfacing sample is shown below in
Figure 2. The average thickness of the sample was measured (on the day of testing) to be approximately 50mm.
Figure 2a & 2b: Photographs of the ““EDPM” Rubber Impact Surface Tile (50mm)” undersurfacing test sample,
showing a top surface view and the sample cross-section view.
The results from drop tests on the ““EDPM” Rubber Impact Surface Tile (50mm)” sample are listed in Table 2.
The results shown in Table 2 should be read in conjunction with the corresponding Test Sheet in Appendix A.
The critical fall height for the ““EDPM” Rubber Impact Surface Tile (50mm)” undersurfacing sample is
The testing of the tiled wet-pour EPDM/recycled rubber product supplied by ImaginationPlay was undertaken
according to the requirements of the Australian Standard: AS/NZS 4422:1996. The outcome of this testing
resulted with the critical fall height (shown below in Table 3) for the product listed.
The following contain the test sheets for:
• “EDPM” Rubber Impact Surface Tile (50mm)
Playground Safety Surface Test Report: ““EDPM” Rubber Impact Surface
Prepared by MECHTEST: 12th June 2008
AS/NZS 4422:1996 specifies testing requirements
to determine the critical fall height for playground
safety surfaces. The critical fall height is determined
by installing the safety surface as specified by the
manufacturer and determining the fall height at
which one of two safety criteria are exceeded; those
criteria are the Head Injury Criterion exceeding
1000, and the maximum acceleration due to the
impact exceeding 200 g. The critical fall height is
determined by dropping an instrumented headform
from various heights onto the surface and measuring
the acceleration due to the impact. Heights tested
include those which produce measurements that
satisfy the relevant criterion and those which exceed
the relevant criterion.
It should be noted that the results reported here
relate specifically to the installation of the product
as specified by the manufacturer below and no
allowance has been made for incorrect installation,
ageing or degradation of the product. These results
should always be used in consultation with the
The critical fall height has been calculated relative
to a nominated piece of equipment and no
assumption has been made about the height of the
user above that equipment. The critical fall height is
quoted to the nearest 0.1 m, rounded down, as
specified in AS/NZS 4422:1996.
The product tested was supplied by
ImaginationPlay, of Hurstbridge, VIC and is
described as ““EDPM” Rubber Impact Surface Tile
(50mm)”. The product sample consisted of a duallayer
rubber tile surfacing test piece, with an
approximate average measured thickness of 50mm.
The test sample consisted of four equal tile pieces
glued together at the edges by the manufacturer,
resulting with a final test piece of approximately
1m×1m in dimension. The testing was conducted at
the Thebarton Campus of the University of
Installation and substrate
The product sample consisted of a single combined
test piece (of dimension 1m x 1m), resting flat
against the substrate, which was a concrete floor.
This product was tested to the requirements for
AS/NZS 4422:1996. The position of the test
locations on the product sample are shown in Figure
A1. Results at locations A,B & C are presented in
Figure A1: Schematic diagram of the test points used.
Air Temperature: 17°C
Surface Temperature: 17°C
The results for the ““EDPM” Rubber Impact
Surface Tile (50mm)” product are displayed in
Table A1 below:
Critical fall height
The calculated critical fall height for this
product is 1.4m, based on the HIC values
measured at the height of 1.5m in the above table.
The 200 g acceleration limit was not exceeded in
Figures A2 and A3 show how the HIC values and
the peak accelerations vary with the minimum fall
Figure A4 shows an actual acceleration trace from
the tests; specifically from the first drop test at a
height of 1.6m.
AS/NZS 4422:1996, Playground surfacing -
Specifications, requirements and test method
T E S T C E R T I F I C A T E
This is to certify that the product sample: ““EDPM” Rubber Impact Surface Tile
(50mm)” playground undersurfacing, produced by ImaginationPlay (as described
in MechTest Report: MT0976), has been assessed according to the impact test
procedure described in Australian/New Zealand Standard: AS/NZS
Tests were conducted on the impact absorption properties of this dual-layer
EPDM / recycled rubber granule product, having an average total thickness of 50
mm (measured on the day of testing). As a result, the following specification was
Product: ““EDPM” Rubber Impact Surface Tile (50mm)”
Test Date: 12th June 2008
Critical fall height: 1.4m.
This page represents a summary of the major findings of the MechTest report: MT0976. For
more detailed information regarding any aspect of the test procedure, the interpretation of test
results or the description details of the product tested, please refer to the MechTest Report:
MT0976 (in its entirety). A copy of this is available upon request from:
PLEASE CONTACT US FOR MORE INFORMATION, PRICING AND SPECIFICATIONS.
YOU CAN ALSO VISIT OUR PLAYGROUND EQUIPMENT SECTION THAT SHOWS HUNDRED'S OF QUALITY INDOOR AND OUTDOOR PLAYGROUND EQUIPMENT DESIGNS.